Transcript of "Regeneration of periodontal tissue bone replacement grafts"
Regeneration ofPeriodontal Tissue:B o n e Re p l a c e m e n tGraftsMark A. Reynolds, DDS, PhD*,Mary Elizabeth Aichelmann-Reidy, DDS,Grishondra L. Branch-Mays, DDS, MS KEYWORDS Bone grafts Periodontal Intrabony Scaffold Regeneration Bone substitutesBone replacement grafts are widely used to promote bone formation and periodontalregeneration. Conventional surgical approaches, such as open flap debridement,provide critical access to evaluate and detoxify root surfaces as well as establishimproved periodontal form and architecture; however, these surgical techniques offeronly limited potential in restoring or reconstituting component periodontal tissues.Bone grafting materials function, in part, as structural scaffolds and matrices forattachment and proliferation of anchorage-dependent osteoblasts (Fig. 1). A widerange of bone grafting materials, including bone grafts and bone graft substitutes,have been applied and evaluated clinically, including autografts, allografts, xeno-grafts, and alloplasts (synthetic/semisynthetic materials). Although not all bone graft-ing materials support the formation of a new periodontal attachment apparatus, thereis conclusive evidence that periodontal regeneration is achievable with bone replace-ment grafts in humans.1 The purpose of this review is to provide an overview of the biologic function and clin-ical application of bone replacement grafts for periodontal regeneration. Emphasis isplaced on the clinical and biologic goals of periodontal regeneration as well asevidence-based treatment outcomes.PERIODONTAL REGENERATION: CLINICAL AND BIOLOGIC GOALSThe biologic goal of periodontal regeneration is restoration of the periodontium to itsoriginal form and function. Periodontal repair is healing of the periodontium by tissue Department of Periodontics, Dental School, University of Maryland, 650 West Baltimore Street, Baltimore, MD 21201, USA * Corresponding author. E-mail address: email@example.com (M.A. Reynolds). Dent Clin N Am 54 (2010) 55–71 doi:10.1016/j.cden.2009.09.003 dental.theclinics.com 0011-8532/09/$ – see front matter ª 2010 Elsevier Inc. All rights reserved.
56 Reynolds et al Fig. 1. Particulate bone grafts function, in part, by providing an osteoconductive matrix and structural framework for new bone formation. Demineralized bone matrix (DBM) also exhibits osteoinductivity. Particulate DBM (260–750 mm) is shown. Electron micrograph (inset) shows complex surface topography of a graft particle (Â3000). that does not fully restore the original functional anatomic and morphologic architec- ture. Following conventional surgical approaches, such as open flap debridement, repair of lost periodontal attachment occurs primarily through formation of a long junc- tional epithelium between the gingival flap and the previously diseased root surface. Epithelium is an efficient tissue for rapid wound repair, in part due to the comparatively high proliferation rate and effective adhesive mechanisms of epithelial cells.2,3 Regen- erative therapy, in contrast, is designed to support regeneration of the attachment apparatus, namely the formation of bone, cementum, and periodontal ligament (Fig. 2). Clinical outcome parameters consistent with successful regenerative therapy include reduced probing depth, increased clinical attachment level, and radiographic evidence of bone fill. At present, conclusive evidence of periodontal regeneration can be provided only through histologic evaluation of treated intraosseous defects using unambiguous reference points along the root surface (see Fig. 2). BONE REPLACEMENT GRAFTS Bone replacement grafts (bone grafts and bone graft substitutes) provide a structural framework for clot development, maturation, and remodeling that supports bone formation in osseous defects. Bone grafting materials also exhibit a variable capacity to promote the coordinated formation of bone, cementum, and periodontal ligament when placed and retained in periodontal defects. Bone grafting materials must possess the attributes of biocompatibility (lacking an immunogenic response) and os- teoconductivity (providing a structure and surface topography that permit cellular attachment, proliferation, and migration). Bone replacement grafts may also possess other properties that support osteogenesis. Osteogenic grafting materials, such as cancellous bone/bone marrow, contain living cells that are capable of differentiation and formation of bone. Osteoinductive grafting materials, such as demineralized bone matrix (DBM), provide a biologic stimulus (proteins and growth factors) that induces the progression of mesenchymal stem cells and other osteoprogenitor cells toward the osteoblast lineage. The Food and Drug Administration (FDA) regulates bone grafting materials that are intended to fill, augment, or reconstruct periodontal or bony defects of the oral and maxillofacial region. The regulatory control of the FDA includes human cells, tissues,
Bone Replacement Grafts 57Fig. 2. Histologic evidence of periodontal regeneration (new bone, cementum, and peri-odontal ligament) following bone grafting with DBM. Note the reference notches (referencepoints for histologic measure of regenerated tissues) placed in the root to mark the pretreat-ment apical extent of calculus (bottom arrow) and height of the alveolar crest (top arrow)(HE, original magnification Â25). (Courtesy of Dr Gerald M. Bowers, Pasadena, MD.)and cellular-based products, under statutes published in Code of Federal Regulations(Federal Register, Title 21) that are intended for transplantation. Multiple classificationsystems have been used to organize bone replacement grafts, which commonlyinclude source (eg, allograft), chemical composition (eg, calcium phosphate), andphysical properties (eg, ceramic). Advances in material sciences, however, haveincreasingly blurred such boundaries between types of bone replacement grafts.For the purposes of this review, bone replacement grafts have been organizedprimarily according to source.AutograftsThe ‘‘gold standard’’ for bone grafting procedures historically has been particulatecancellous bone/bone marrow autografts, which can provide a rich source of boneand marrow cells that have osteogenic potential. Histologic findings from case reportssubstantiate the potential for autogenous bone/bone marrow grafts to support peri-odontal regeneration in humans.4,5 Multiple clinical considerations have limited theuse of extraoral autografts, particularly from iliac crest, including the possibility ofsurgical complications and pain associated with donor site. Autogenous bone is frequently harvested from intraoral sites, often from the samequadrant as the regenerative surgery. Intraoral donor sites, however, typically yieldcomparatively limited graft volume. Harvesting sufficient donor bone, therefore, asan osseous coagulum of cortical or cortical-cancellous bone, can necessitate thecreation of additional intraoral surgical sites, thereby increasing the potential forsurgical morbidity and discomfort.
58 Reynolds et al Allografts Bone allograft is the most frequently used alternative to autogenous bone for bone grafting procedures in the United States. Under FDA regulations, facilities engaged in procuring and processing human tissues for transplantation must ensure that spec- ified minimum medical screening and infectious disease testing have been performed, and that records exist and are maintained to document screening and testing for each human tissue. The American Association of Tissue Banks also sets standards, inspects facilities, and accredits tissue banks in North America. There are no reports of disease transmission during the 30-year history of use of freeze-dried bone allo- grafts in periodontal therapy.6 Tissue banks process bone allografts using a variety of methods, some based on proprietary techniques, but most are based on similar underlying concepts that address cleansing, decontamination, antimicrobial treatment, dehydration, graft size, and terminal sterilization.7 Particulate bone allografts are provided as mineralized or demineralized products. Allogeneic bone that has undergone extensive demineral- ization is referred to as DBM or demineralized freeze-dried bone allograft (DFDBA). DBM exhibits the capacity to induce bone formation in nonorthotopic sites, such as muscle, and is considered to be osteoinductive. Bone demineralized to levels of approximately 2% residual calcium has been shown to provide maximum osteoinduc- tive potential by assay systems,8 presumably due to exposure of bone morphogenetic proteins.9 Bowers and colleagues10,11 have provided conclusive histologic evidence that DBM supports periodontal regeneration in humans. Xenografts Xenografts are surgical grafts transplanted between different species. Two sources of xenografts are commercially marketed as particulate bone replacement grafts in clinical practice: bovine bone and natural coral. Anorganic bovine bone graft (ABM) is a naturally derived porous and deproteinized bovine bone mineral with comparable mineral composition and microporous structure to native humane bone.12–15 ABM has been shown to support significant gains in clinical attachment level and hard tissue fill in human intrabony defects.16 Available human histologic evidence provides proof-of- principle evidence that ABM17 and ABM/collagen18 can support periodontal regener- ation in intrabony defects. The calcium carbonate exoskeleton of coral species, such as Porites, can be con- verted to hydroxyapatite by hydrothermal exchange. Calcium carbonate-hydroxyap- atite constructs can be produced by limited hydrothermal conversion.19 The porosity and pore size distribution of hydroxyapatite, which is dependent primarily on coral species, provides a osteoconductive scaffold that enhances bone forma- tion20 and undergoes dissolution and resorption with bone remodeling.21,22 Ripamonti and colleagues19,23–26 have shown that coral-derived biomimetic matrices of different chemical compositions have the capacity to induce heterotopic bone formation in the nonhuman primate Papio ursinus. Alloplasts An alloplast is a biocompatible, inorganic synthetic bone grafting material. At present, alloplasts marketed for periodontal regeneration fall into 2 broad classes: ceramics and polymers. The composition, morphology, and surface topography of alloplasts provide the osteoconductive platform for promoting bone formation along the surface of the grafting material.27 The fate of an alloplastic bone grafting material is dependent primarily on its chemical composition, structure, and physical properties.
Bone Replacement Grafts 59 Ceramic-based bone grafting materials have been widely used for bone and peri-odontal regeneration, and function primarily through osteoconduction. Commerciallyavailable ceramic-based materials include calcium phosphates (eg, tricalcium phos-phate and hydroxyapatite), calcium sulfate, and bioactive glass. These ceramicshave also been considered osteointegrative,27 because of the tenacious, intimatebond formed between the new mineralized tissue and graft material.28 Ceramicscan exist in fully amorphous or crystalline phases, with the same ratios of elementalsubstances (calcium and phosphorus). Differences in the degree of crystallinearrangement significantly impact the physical and biologic characteristics of theceramic, including strength, modulus, and dissolution rate.29 Synthetic and coral-derived porous hydroxyapatite has been shown to supportsignificant clinical improvements in periodontal measures following implantation in in-trabony defects.1 The porosity and degree of sintering of synthetic hydroxyapatiteceramics primarily determines the rate of biodegradation—crystalline, nonporoushydroxyapatite is essentially nondegradable.30 Human histologic evidence of ossifica-tion of the graft pores and the graft periphery of porous hydroxyapatite has been foundin periodontal intrabony sites, with residual graft particles present 12 months followingimplantation.31 Porous hydroxyapatite appears to exhibit osteoconductive properties,as reflected clinically in bone formation; however, no evidence of periodontal regener-ation has been shown. b-Tricalcium phosphate (b-TCP) is a porous form of calcium phosphate, with similarproportions of calcium and phosphate to cancellous bone.32 As a bone grafting mate-rial, b-TCP supports improvements in clinical outcomes, including clinical attachmentlevel, but histologic evidence reveals periodontal repair, primarily through the forma-tion of a long junctional epithelial attachment, with limited new connective tissueattachment.33–35 Although the surface layer of b-TCP allows for bone deposition inorthopedic sites,28 including maxillary sinus augmentation,36 this ceramic has beenshown to become fibroencapsulated when placed in periodontal intrabony defects,failing to stimulate new bone growth, with residual graft particles evident 18 monthsfollowing treatment.33–35 Differences in the stoichiometric chemistry and structure ofb-TCP may affect the rate of resorption and replacement with bone during healing.36 Bioactive glass is a ceramic composed principally of SiO2. The original compositionof bioactive glass approved by the FDA, designated 45S5, was composed of 46.1mol% SiO2, 26.9 mol% CaO, 24.4 mol% Na2O, and 2.5 mol% P2O5.37 The originalcomposition and fine structure has been extensively modified in an attempt to furtherenhance bioactive glass as a bone replacement graft. Bioglass can bond directly tobone through the development of a surface layer of carbonated hydroxyapatite insitu.37 This calcium phosphate-rich layer is thought to promote adsorption andconcentration of osteoblast-derived proteins necessary for the mineralization of extra-cellular matrix.38 Bioactive glass has been shown to significantly increase clinicalattachment level and hard tissue fill when implanted in intrabony defects.1 Althoughbioactive glass exhibits osteconductive properties as a grafting material in maxillarysinus39,40 and extraction socket,41–43 histologic analysis of human periodontal defectshas revealed healing primarily by connective tissue encapsulation of the graft materialand epithelial down-growth, with minimal evidence of new cementum or connectivetissue attachment limited to the most apical part of the defect.44,45 Polymers can be classified based on source: natural and synthetic. Natural poly-mers that have been used in the fabrication of bone grafting materials include polysac-charides (eg, agarose, alginate, hyaluronic acid, chitosan) and polypeptides (eg,collagen, gelatin); however, the structural properties of natural polymers, includinga comparatively weak mechanical strength and variable rates of degradation,46
60 Reynolds et al have limited their use as standalone bone grafting materials. Natural polymers may serve an important role in composite grafts, which incorporate a particulate or bio- logic, such as Bio-Oss Collagen (Geistlich Pharma AG, Wolhusen, Switzlerland). Synthetic polymers (eg, poly(glycolic acid), poly(L-lactic acid), polyorthoester, poly- anhydride) provide a platform for controlling the biomechanical properties of scaffolds as well as targeting drug delivery in tissue engineering.47 Polymers are more widely used as barrier materials in guided tissue regeneration (GTR) procedures for the treat- ment of periodontal defects. At present, several polymer systems are being used for bone and periodontal regeneration, including polylactic acid (PLA)-based polymers and copolymers. These polymers have proved to be effective in periodontal applica- tions as barrier materials48 but can elicit inflammatory and foreign body reactions, especially following fragmentation secondary to bulk degradation.49,50 Synthetic poly- mers have an expanded use in orthopedic applications as injectable and solid resin- based products.27 At present, a biocompatible microporous polymer containing polymethylmethacrylate (PMMA), polyhydroxylethylmethacrylate (PHEMA), and calcium hydroxide is available as a bone grafting material for the treatment of periodontal defects. This composite is prepared from a core of PMMA and PHEMA with a coating of calcium hydroxide. The polymer is hydrophilic and osteophilic, which purportedly aids in stabilization of the heal- ing clot. A controlled study51 and case series reports52–55 provide evidence for the effec- tiveness of this polymeric grafting material in improving clinical parameters, relative to open flap debridement, in the treatment of periodontal intraosseous defects.51 Histo- logic evaluations revealed that the polymer was associated with minimal inflammation and infrequent foreign body giant cells, with evidence of both bone apposition and soft tissue encapsulation, at 1 to 30 months following implantation.51,55–57 COMPOSITE GRAFTS In periodontal regenerative procedures, bone replacement grafts have been widely used to expand the volume of autogenous bone for regenerative procedures when sufficient autogenous bone is not readily available. The bone replacement graft, there- fore, serves as a graft expander or extender. In other regenerative applications, such as ridge and sinus augmentation whereby structural support is often necessary, the physical properties of the graft expander can be an important factor in regenerative outcome. Anorganic bovine graft material, for example, provides a stable osteocon- ductive structural framework or matrix for bone in-growth and undergoes minimal degradation and remodeling over comparatively long periods.58–60 Recent advances in material sciences now permit the fabrication of polymeric and ceramic composite grafts, with biologic and physical properties optimized for specific tissue engineering applications.61 Strategies to improve the delivery and containment of bone replacement grafts have focused on agents that function as a graft carriers or binders. Human histologic evidence has shown that the presence of residual DBM particles is closely associated with the extent of periodontal regeneration.62 Most carriers are solid gels or pastes, which are designed to resorb within several days of implantation. Carrier materials used in commercially marketed DBM-based products include Poloxamer 407, lecithin, hyaluronic acid, glycerol, porcine gelatin, and calcium sulfate, among others.63 These carrier materials impart different properties to the particulate bone grafting material. Poloxamer 407, for example, is a reverse-phase polymer that is fluid at room temper- ature and becomes a firm gel at body temperature. In orthopedic applications, carrier
Bone Replacement Grafts 61materials have been implicated in differences in the efficacy64 and potential safety ofDBM products.65,66BIOMIMETICS AND BIOLOGICSOsteoblasts are anchorage-dependent cells that are highly responsive to the surfacecharacteristics of osteoconductive scaffolds. Efforts to enhance the effectiveness ofgraft materials have focused on the use of biomimetic engineering and biologicagents, such as growth factors. PepGen P-15 (Dentsply Friadent, Mannheim,Germany) is bovine-derived hydroxyapatite (anorganic bone) that contains a shortpolypeptide chain of 15 amino acids, which is a biomimetic cell-binding region oftype I collagen. The amino acid peptide, therefore, mimics type I collagen, the majorcomponent of bone matrix, promoting cell attachment, which may enhance osteogen-esis. In vitro studies have shown that ABM carrying the cell-binding peptide P-15promotes anchorage-dependent cell survival.12 The efficacy of PepGen P-15 for thetreatment of intrabony defects has been established in controlled clinical trials.67,68 The potential for growth factors to modify and enhance the regenerative capacity ofbone grafts was highlighted in early studies examining the osteoinductive properties ofDBM. Recent attention has focused on the potential for biologic mediators to improvewound healing and enhance the clinical benefits of bone replacement grafts. Platelet-rich plasma (PRP), collected by centrifugation of autogenous serum, provides a sourceof highly concentrated platelets, which produce growth factors that are critical fornormal healing. When admixed with a bone graft, PRP facilitates graft placementand containment (Fig. 3). PRP has been shown to provide beneficial effects, as re-flected in gains in clinical attachment level, when used as an adjunct to periodontalregenerative therapy.69 In 2005, the FDA approved for marketing a new dental bone filling device, GEM 21S(Osteohealth/Luitpold Pharmaceuticals, Inc, Shirley, NY), which combines recombi-nant human platelet-derived growth factor-BB (rhPDGF-BB) and b-TCP for the treat-ment of periodontal-related defects. GEM 21S is a completely synthetic graftingsystem and is the first dental bone grafting material with a recombinant growth factorapproved by the FDA. GEM 21S contains over 1000 times the concentration ofplatelet-derived growth factor obtainable in current PRP preparations from thepatient’s own peripheral venous blood. PDGF-BB promotes angiogenesis as well asenhances cell recruitment and proliferation of bone and periodontal ligament cells.70,71Fig. 3. Platelet-rich plasma provides a source of autogenous growth factors and can facili-tate graft placement and containment. (Courtesy of Dr James D. Kassolis, Baltimore, MD.)
62 Reynolds et al The efficacy and safety of GEM 21S for the treatment of intrabony defects has been established in a large-scale multicenter, randomized controlled clinical trial.72 BONE GRAFT THERAPY Surgery Bone graft therapy builds on the basic principles of periodontal surgical technique, including appropriate case selection and preoperative management. Complete defect debridement and root surface decontamination are essential before placement of the bone graft material. The most notable difference in surgical technique involves gingival flap design, because primary and passive flap closure are critical for ensuring wound closure. In general, full-thickness mucoperiosteal flaps are elevated using sulcular incisions to conserve the papillary and keratinized tissue, ensuring the flap can be adapted at a more coronal level postoperatively. This procedure will aid the develop- ment of space for the graft material and stability of the healing clot at a more coronal level than the prior diseased attachment level. The flap design, when possible, ideally avoids placing an incision directly over the defect site, because the defect site does not provide direct periosteal blood supply and lacks optimal structural support of the incision margins. Following thorough root debridement and preparation of the defect site under magnification and supplemental illumination, the bone grafting mate- rial is implanted into the defect, lightly condensed, and contoured to mimic the normal architecture of adjacent alveolar process. The mucoperiosteal flaps are mobilized to permit tension-free coaptation and primary closure with sutures (Fig. 4). The most commonly reported untoward event following bone graft therapy in controlled clinical trials has been partial loss (exfoliation) of graft particles postoperatively.1 Evidence of retained or residual DBM graft particles has been shown to be closely associated with the extent of periodontal regeneration in histologic analysis.62 Root Surface Biomodification The topical application of chemical agents to modify the root surface is among one of the earliest reported clinical approaches to prepare root surfaces for optimal attach- ment of periodontal tissues and regeneration.73 Several agents, such as citric acid, tetracycline, and ethylenediamine tetra-acetic acid (EDTA), have been shown to result in surface biomodification, including detoxification, demineralization, and collagen fiber exposure. A recent systematic review, however, concluded that chemical root modifiers do not enhance reductions in probing depth or gains in clinical attachment level following periodontal surgery.74 Because improvements in clinical measures can occur following periodontal repair—via a long junctional epithelium, connective tissue attachment, or both—as well as periodontal regeneration, many clinicians continue to routinely apply root modifiers in an effort to promote true regeneration, namely the formation of new bone, cementum, and periodontal ligament. PERIODONTAL DEFECTS AND REGENERATIVE SUCCESS Periodontitis results in destructive changes in the component hard and soft tissues of the periodontium, culminating in loss of supporting alveolar bone and periodontal attachment. Horizontal patterns of alveolar bone loss are not amenable to periodontal regeneration with current regenerative therapies, including bone grafts. Vertical or angular bony defects, including furcation defects, are often responsive to periodontal regeneration.
63Fig. 4. (A) Mandibular left second molar presents with periodontal pocketing on the directdistal. Patient is a nonsmoker and demonstrates excellent oral hygiene. (Courtesy of Dr PaulS. Rosen, Yardley, PA.) (B) Preoperative radiograph reveals evidence of an advanced intrab-ony defect on the distal aspect of the tooth. (C) Elevation of facial and lingual flaps usingsulcular incisions, preserving the papilla, exposes a 3-wall intrabony defect measuring 6mm from base to the alveolar crest on the distal of the second molar. Rotary instrumenta-tion using a multifluted surgical length burr was used to plane the root surface to the depthof the defect. Small perforations are made to decorticate the bony walls of the defect, fol-lowed by the topical application of citric acid (pH 1.0) to decontaminate and condition theroot surface. (D) Mineralized freeze-dried bone allograft admixed with calcium sulfate isplaced with light incremental pressure until the bone graft slightly overfills of the defect.(E) Primary closure of the flaps is achieved using expanded polytetrafluoroethylene sutures(Gore-Tex; W.L. Gore and Associates, Inc, Newark, DE). (F) Clinical presentation of thesurgical site 1 year following bone grafting surgery. (G) Postoperative radiograph suggestsremodeling of the graft with nearly complete resolution of the intrabony defect.
64 Reynolds et al Intrabony Defects Intrabony defects are commonly described by the number of bony walls (1, 2, or 3 walls) and depth of the defect (measured from the crestal height of bone to the base of the defect) (Fig. 5). Periodontal probing and transgingival bone ‘‘sounding’’ can provide important diagnostic information to aid the appropriate selection of regen- erative therapy for intrabony defects.75 Radiographs also provide important diag- nostic information related to defect morphology but generally underestimate the severity of bone loss.76 Furcation Defects Furcation invasion is most commonly classified according to the degree of horizontal extension within the furcation. The degree of furcation involvement is often classified as Class I (incipient loss of bone limited to the furcation flute that does not extend hor- izontally within the furcation), Class II (variable bone loss that does not extend completely through the furcation), and Class III (bone loss extending completely through the furcation).77 Although early or incipient Class I furcation defects are generally considered main- tainable by nonsurgical therapy and effective plaque control, more advanced furcation defects (Class II and Class III) usually require surgical management for effective inflam- matory disease control and tooth retention.77 Surgery permits access for root debride- ment, detoxification, and odontoplasty to promote periodontal regeneration. The primary clinical objective in the regenerative treatment of Class II furcation defects is closure of the furcation entrance to the oral environment. Class III furcation defects are generally not amenable to successful regenerative therapy, and are usually treated with surgical debridement and apical positioning of the flap to obtain pocket Fig. 5. Schematic illustration of intraosseous defects classified according to the number of bony walls present. (A) Three-wall defect; (B) 2-wall defect; (C) combination defect; (D) 1-wall defect. One-wall defects typically do not respond well to regenerative therapy.
Bone Replacement Grafts 65reduction, thereby facilitating access for plaque control, or hemisection of the tooth toeliminate the furcation.CASE SELECTIONIn general, early or shallow intrabony lesions (defects of 3 mm or less) and Class I(incipient) furcation defects can be effectively managed using nonsurgical or nonrege-nerative surgical therapies. Early intrabony defects are thought to have less potentialfor regeneration due, in part, to a limited potential for space development for holdinggraft particles and concomitant crestal bone resorption during healing.78 Givenadequate surgical access, the most predictable regenerative outcomes are typicallyachieved in narrow 3-wall defects79 as well as Class II furcation defects with proximalbone height at or above the level of the furcation entrance.80TREATMENT OUTCOMES: EXPECTATIONS BASED ON EVIDENCE-BASED REVIEWSIntrabony DefectsSystematic reviews of randomized controlled trials provide strong evidence that bonereplacement grafts support improvements in clinical parameters, including probingdepth, clinical attachment level, and defect fill, when compared with open flapdebridement alone in intrabony defects (Table 1).1,81–83 Literature-based estimatesof bone fill range from 2.3 to 3.0 mm or 60% of the defect following grafting of intrab-ony defects.84 Particulate bone grafting materials also seem to reduce crestal boneloss, whereas barrier materials may increase recession of the gingival margin.1,48When particulate graft is combined with a barrier, modest but nonsignificant improve-ment in bone levels is obtained, with significant attachment level gain and probingdepth reduction when compared with graft alone.1 Comparisons in treatment outcomes, such as defect fill, obtained in differentstudies must be made with caution. Laurell and colleagues78 reviewed all observa-tional and controlled studies published during a 20-year period on the surgical treat-ment of intrabony defects with open flap debridement, GTR, and bone grafts. Defect Table 1 Mean change in clinical measures following bone replacement graft therapy Bone Clinical Replacement Attachment Probing Graft N Level (mm) N Depth (mm) N Defect Fill (mm) Allograft 12 1.6 Æ 1.3 10 2.9 Æ 1.6 13 2.2 Æ 1.4 Autograft 3 2.6 Æ 1.2 1 1.4 Æ 1.0 2 2.2 Æ 1.2 Synthetic 4 2.8 Æ 1.7 7 3.2 Æ 1.4 6 2.1 Æ 1.3 hydroxyapatite Coralline 4 2.3 Æ 1.4 4 3.2 Æ 1.5 3 2.8 Æ 1.2 hydroxyapatite Bioactive glass 4 2.3 Æ 1.8 4 3.4 Æ 1.8 4 2.6 Æ 1.0 PepGen P-15 1 1.3 Æ 1.9 1 2.4 Æ 1.5 1 2.8 Æ 1.2 GEM 21S 1 3.7 Æ 0.2 1 4.4 Æ 0.2 1 2.5 Æ 0.3aValues represent mean Æ standard deviation, where N 5 number of studies. Summary statistics are derived from randomized controlled studies. Reported in Reynolds et al1(allograft, autograft, synthetic hydroxyapatite, coralline hydroxyapatite, bioactive glass); Yukna etal67 (PepGen P-15); Nevins et al93 (GEM 21S). a Hard tissue measurements by radiographic assessment.
66 Reynolds et al fill was found to be positively correlated with initial defect depth following open flap debridement and grafting procedures, as reported by others. Differences in mean defect fill parallel initial differences in average pretreatment defect depth, making direct quantitative comparisons of improvements (effect sizes) across studies difficult to evaluate and vulnerable to confounding. Histologic evidence of periodontal regeneration in intraosseous defects has been re- ported most extensively for autogenous bone and DFDBA, although case reports provide proof-of-principle of regeneration for other bone grafting materials, such as PepGen P-15,85 Bio-Oss Collagen (anorganic bovine-derived bone matrix and collagen),86 and GEM 21S.87 In contrast, open flap debridement and alloplastic grafts support primarily periodontal repair, which is characterized by formation of a long junctional epithelium.1 Furcation Defects Systematic reviews provide strong evidence that Class II furcations respond most favorably and predictably to a combinatorial approach using GTR and a bone grafting material together.48 Using this combination therapy, Bowers and colleagues80 achieved the highest rate of complete furcation closure in mandibular molar Class II facial defects, with horizontal probing depths of 5 mm or less and interproximal bone at or above the level of the furcation entrance. In general, the more advanced the furcation defect, the less favorable the prognosis for complete periodontal regen- eration and furcation closure. Early treatment of furcation defects, therefore, is critical for improving the overall prognosis. FACTORS IMPACTING TREATMENT OUTCOME The success of regenerative therapy is influenced by multiple factors related to the patient, periodontal defect, and surgical management,88,89 which contribute to vari- ability in clinical outcomes following regenerative therapy.90 Defect morphology and root configuration can affect both surgical access and containment of the bone replacement graft, thereby influencing treatment outcome. Patient compliance with recommended oral hygiene procedures and supportive periodontal maintenance programs are essential for achieving an optimal regenerative outcome and long- term therapeutic success. Finally, smoking adversely affects wound healing, including periodontal regeneration, and increases the risk for periodontal breakdown following treatment.91,92 SUMMARY Controlled clinical trials provide strong evidence for the effectiveness of bone replace- ment grafts in the treatment of periodontal defects. The potential for selected bone replacement grafts, such as DBM, to support true periodontal regeneration, including new bone, cementum, and periodontal ligament, has been well established through histologic analysis in humans. Most current bone grafting materials are osteoconduc- tive and function as passive matrices for ingrowth of osteoprogenitor tissue. Composite grafting materials, incorporating biomimetic and biologic components, have shown great potential to enhance regenerative outcomes. Future bone grafting materials will likely build on innovative polymeric and ceramic platforms with controlled biophysical properties that enable the targeted delivery of drugs, biologics, and cells, thereby improving the degree and predictability of periodontal regeneration.
Bone Replacement Grafts 67REFERENCES 1. Reynolds MA, Aichelmann-Reidy ME, Branch-Mays GL, et al. The efficacy of bone replacement grafts in the treatment of periodontal osseous defects. A systematic review. Ann Periodontol 2003;8:227. 2. Shimono M, Ishikawa T, Enokiya Y, et al. Biological characteristics of the junc- tional epithelium. J Electron Microsc (Tokyo) 2003;52:627. 3. Nievers MG, Schaapveld RQ, Sonnenberg A. Biology and function of hemides- mosomes. Matrix Biol 1999;18:5. 4. Hiatt WH, Schallhorn RG, Aaronian AJ. The induction of new bone and cementum formation. IV. Microscopic examination of the periodontium following human bone and marrow allograft, autograft and nongraft periodontal regenerative proce- dures. J Periodontol 1978;49:495. 5. Ross SE, Cohen DW. The fate of a free osseous tissue autograft. A clinical and histologic case report. Periodontics 1968;6:145. 6. Centers for Disease Control and Prevention: Bone allografts. What is the risk of disease transmission with bone allografts? In: Department of Health and Human Services. Available at: http://www.cd.gov/OralHealth/Infectioncontrol/faq/allografts. htm. Accessed September 30, 2009. 7. Holtzclaw D, Toscano N, Eisenlohr L, et al. The safety of bone allografts used in dentistry: a review. J Am Dent Assoc 2008;139:1192. 8. Zhang M, Powers RM Jr, Wolfinbarger L Jr. Effect(s) of the demineralization process on the osteoinductivity of demineralized bone matrix. J Periodontol 1997;68:1085. 9. Urist MR. Bone: formation by autoinduction. Science 1965;150:893.10. Bowers G, Felton F, Middleton C, et al. Histologic comparison of regeneration in human intrabony defects when osteogenin is combined with demineralized freeze- dried bone allograft and with purified bovine collagen. J Periodontol 1991;62:690.11. Bowers GM, Chadroff B, Carnevale R, et al. Histologic evaluation of new attach- ment apparatus formation in humans. Part III. J Periodontol 1989;60:683.12. Hanks T, Atkinson BL. Comparison of cell viability on anorganic bone matrix with or without P-15 cell binding peptide. Biomaterials 2004;25:4831.13. Rosen VB, Hobbs LW, Spector M. The ultrastructure of anorganic bovine bone and selected synthetic hyroxyapatites used as bone graft substitute materials. Biomaterials 2002;23:921.14. Fulmer NL, Bussard GM, Gampper TJ, et al. Anorganic bovine bone and analogs of bone mineral as implants for craniofacial surgery: a literature review. J Long Term Eff Med Implants 1998;8:69.15. Spector M. Anorganic bovine bone and ceramic analogs of bone mineral as implants to facilitate bone regeneration. Clin Plast Surg 1994;21:437.16. Richardson CR, Mellonig JT, Brunsvold MA, et al. Clinical evaluation of Bio-Oss: a bovine-derived xenograft for the treatment of periodontal osseous defects in humans. J Clin Periodontol 1999;26:421.17. Mellonig JT. Human histologic evaluation of a bovine-derived bone xenograft in the treatment of periodontal osseous defects. Int J Periodontics Restorative Dent 2000;20:19.18. Nevins ML, Camelo M, Lynch SE, et al. Evaluation of periodontal regeneration following grafting intrabony defects with bio-oss collagen: a human histologic report. Int J Periodontics Restorative Dent 2003;23:9.19. Ripamonti U, Crooks J, Khoali L, et al. The induction of bone formation by coral- derived calcium carbonate/hydroxyapatite constructs. Biomaterials 2009;30: 1428.
68 Reynolds et al 20. Damien E, Revell PA. Coralline hydroxyapatite bone graft substitute: a review of experi- mental studies and biomedical applications. J Appl Biomat Biomech 2004;2:65. 21. Guillemin G, Meunier A, Dallant P, et al. Comparison of coral resorption and bone apposition with two natural corals of different porosities. J Biomed Mater Res 1989;23:765. 22. Guillemin G, Patat JL, Fournie J, et al. The use of coral as a bone graft substitute. J Biomed Mater Res 1987;21:557. 23. Ripamonti U. The morphogenesis of bone in replicas of porous hydroxyapatite obtained from conversion of calcium carbonate exoskeletons of coral. J Bone Joint Surg Am 1991;73:692. 24. Ripamonti U. Calvarial reconstruction in baboons with porous hydroxyapatite. J Craniofac Surg 1992;3:149. 25. Ripamonti U. Osteoinduction in porous hydroxyapatite implanted in heterotopic sites of different animal models. Biomaterials 1996;17:31. 26. Ripamonti U, Van den Heever B, Van Wyk J. Expression of the osteogenic pheno- type in porous hydroxyapatite implanted extraskeletally in baboons. Matrix 1993; 13:491. 27. Laurencin C, Khan Y, El-Amin SF. Bone graft substitutes. Expert Rev Med Devices 2006;3:49. 28. Boccaccini AR, Blaker JJ. Bioactive composite materials for tissue engineering scaffolds. Expert Rev Med Devices 2005;2:303. 29. Lemons JE. Bioceramics. Is there a difference? Clin Orthop Relat Res 1990;261: 153. 30. Klein CP, Driessen AA, de Groot K, et al. Biodegradation behavior of various calcium phosphate materials in bone tissue. J Biomed Mater Res 1983;17:769. 31. Stahl SS, Froum SJ. Histologic and clinical responses to porous hydroxylapatite implants in human periodontal defects. Three to twelve months postimplantation. J Periodontol 1987;58:689. 32. Hashimoto-Uoshima M, Ishikawa I, Kinoshita A, et al. Clinical and histologic observation of replacement of biphasic calcium phosphate by bone tissue in monkeys. Int J Periodontics Restorative Dent 1995;15:205. 33. Baldock WT, Hutchens LH Jr, McFall WT Jr, et al. An evaluation of tricalcium phos- phate implants in human periodontal osseous defects of two patients. J Periodon- tol 1985;56:1. 34. Stahl SS, Froum S. Histological evaluation of human intraosseous healing responses to the placement of tricalcium phosphate ceramic implants. I. Three to eight months. J Periodontol 1986;57:211. 35. Froum S, Stahl SS. Human intraosseous healing responses to the placement of tricalcium phosphate ceramic implants. II. 13 to 18 months. J Periodontol 1987; 58:103. 36. Chopra PM, Johnson M, Nagy TR, et al. Micro-computed tomographic analysis of bone healing subsequent to graft placement. J Biomed Mater Res B Appl Biomater 2009;88:611. 37. Hench LL, Paschall HA. Direct chemical bond of bioactive glass-ceramic materials to bone and muscle. J Biomed Mater Res 1973;7:25. 38. Schepers E, de Clercq M, Ducheyne P, et al. Bioactive glass particulate material as a filler for bone lesions. J Oral Rehabil 1991;18:439. 39. Galindo-Moreno P, Avila G, Fernandez-Barbero JE, et al. Clinical and histologic comparison of two different composite grafts for sinus augmentation: a pilot clinical trial. Clin Oral Implants Res 2008;19:755.
Bone Replacement Grafts 6940. Scarano A, Degidi M, Iezzi G, et al. Maxillary sinus augmentation with different biomaterials: a comparative histologic and histomorphometric study in man. Implant Dent 2006;15:197.41. Stvrtecky R, Gorustovich A, Perio C, et al. A histologic study of bone response to bioactive glass particles used before implant placement: a clinical report. J Pros- thet Dent 2003;90:424.42. Norton MR, Wilson J. Dental implants placed in extraction sites implanted with bioactive glass: human histology and clinical outcome. Int J Oral Maxillofac Implants 2002;17:249.43. Froum S, Cho SC, Rosenberg E, et al. Histological comparison of healing extrac- tion sockets implanted with bioactive glass or demineralized freeze-dried bone allograft: a pilot study. J Periodontol 2002;73:94.44. Nevins ML, Camelo M, Nevins M, et al. Human histologic evaluation of bioactive ceramic in the treatment of periodontal osseous defects. Int J Periodontics Restorative Dent 2000;20:458.45. Sculean A, Windisch P, Keglevich T, et al. Clinical and histologic evaluation of an enamel matrix protein derivative combined with a bioactive glass for the treat- ment of intrabony periodontal defects in humans. Int J Periodontics Restorative Dent 2005;25:139.46. Lee K, Kaplan D, editors. Tissue engineering I. Scaffold systems for tissue engi- neering, Advances in biochemical engineering/biotechnology, vol. 102. New York: Springer; 2006.47. Sokolsky-Papkov M, Agashi K, Olaye A, et al. Polymer carriers for drug delivery in tissue engineering. Adv Drug Deliv Rev 2007;59:187.48. Murphy KG, Gunsolley JC. Guided tissue regeneration for the treatment of peri- odontal intrabony and furcation defects. A systematic review. Ann Periodontol 2003;8:266.49. Polimeni G, Koo KT, Pringle GA, et al. Histopathological observations of a polylac- tic acid-based device intended for guided bone/tissue regeneration. Clin Implant Dent Relat Res 2008;10:99.50. Danesh-Meyer MJ, Wikesjo UM. Gingival recession defects and guided tissue regeneration: a review. J Periodont Res 2001;36:341.51. Yukna RA. HTR polymer grafts in human periodontal osseous defects. I. 6-month clinical results. J Periodontol 1990;61:633.52. Calongne KB, Aichelmann-Reidy ME, Yukna RA, et al. Clinical comparison of microporous biocompatible composite of PMMA, PHEMA and calcium hydroxide grafts and expanded polytetrafluoroethylene barrier membranes in human mandibular molar Class II furcations. A case series. J Periodontol 2001;72:1451.53. Haris AG, Szabo G, Ashman A, et al. Five-year 224-patient prospective histolog- ical study of clinical applications using a synthetic bone alloplast. Implant Dent 1998;7:287.54. Yukna RA, Yukna CN. Six-year clinical evaluation of HTR synthetic bone grafts in human grade II molar furcations. J Periodont Res 1997;32:627.55. Yukna RA, Greer RO Jr. Human gingival tissue response to HTR polymer. J Biomed Mater Res 1992;26:517.56. Stahl SS, Froum SJ, Tarnow D. Human clinical and histologic responses to the placement of HTR polymer particles in 11 intrabony lesions. J Periodontol 1990;61:269.57. Froum SJ. Human histologic evaluation of HTR polymer and freeze-dried bone allograft. A case report. J Clin Periodontol 1996;23:615.
70 Reynolds et al 58. Iezzi G, Scarano A, Mangano C, et al. Histologic results from a human implant retrieved due to fracture 5 years after insertion in a sinus augmented with anorganic bovine bone. J Periodontol 2008;79:192. 59. Traini T, Valentini P, Iezzi G, et al. A histologic and histomorphometric evaluation of anorganic bovine bone retrieved 9 years after a sinus augmentation proce- dure. J Periodontol 2007;78:955. 60. Sartori S, Silvestri M, Forni F, et al. Ten-year follow-up in a maxillary sinus augmen- tation using anorganic bovine bone (Bio-Oss). A case report with histomorpho- metric evaluation. Clin Oral Implants Res 2003;14:369. 61. Hutmacher DW, Schantz JT, Lam CX, et al. State of the art and future directions of scaffold-based bone engineering from a biomaterials perspective. J Tissue Eng Regen Med 2007;1:245. 62. Reynolds MA, Bowers GM. Fate of demineralized freeze-dried bone allografts in human intrabony defects. J Periodontol 1996;67:150. 63. Borden M. The development of bone graft materials using various formulations of demineralized bone matrix. In: Laurencin CT, editor. Bone graft substitutes. West Conshohocken (PA): ASTM International. 2003. Chapter 5. p. 96 64. Drosos GI, Kazakos KI, Kouzoumpasis P, et al. Safety and efficacy of commer- cially available demineralised bone matrix preparations: a critical review of clinical studies. Injury 2007;38(Suppl 4):S13. 65. Wang JC, Kanim LE, Nagakawa IS, et al. Dose-dependent toxicity of a commer- cially available demineralized bone matrix material. Spine (Phila Pa 1976) 2001; 26:1429. 66. Bostrom MP, Yang X, Kennan M, et al. An unexpected outcome during testing of commercially available demineralized bone graft materials: how safe are the nonallograft components? Spine (Phila Pa 1976) 2001;26:1425. 67. Yukna RA, Callan DP, Krauser JT, et al. Multi-center clinical evaluation of combi- nation anorganic bovine-derived hydroxyapatite matrix (ABM)/cell binding peptide (P-15) as a bone replacement graft material in human periodontal osseous defects. 6-month results. J Periodontol 1998;69:655. 68. Yukna RA, Krauser JT, Callan DP, et al. Multi-center clinical comparison of combi- nation anorganic bovine-derived hydroxyapatite matrix (ABM)/cell binding peptide (P-15) and ABM in human periodontal osseous defects. 6-month results. J Periodontol 2000;71:1671. 69. Plachokova AS, Nikolidakis D, Mulder J, et al. Effect of platelet-rich plasma on bone regeneration in dentistry: a systematic review. Clin Oral Implants Res 2008;19:539. 70. Hollinger JO, Hart CE, Hirsch SN, et al. Recombinant human platelet-derived growth factor: biology and clinical applications. J Bone Joint Surg Am 2008; 90(Suppl 1):48. 71. Oates TW, Rouse CA, Cochran DL. Mitogenic effects of growth factors on human periodontal ligament cells in vitro. J Periodontol 1993;64:142. 72. Nevins M, Camelo M, Nevins ML, et al. Periodontal regeneration in humans using recombinant human platelet-derived growth factor-BB (rhPDGF-BB) and allo- genic bone. J Periodontol 2003;74:1282. 73. Lowenguth RA, Blieden TM. Periodontal regeneration: root surface demineraliza- tion. Periodontol 2000 1993;1:54. 74. Mariotti A. Efficacy of chemical root surface modifiers in the treatment of periodontal disease. A systematic review. Ann Periodontol 2003;8:205. 75. Kim HY, Yi SW, Choi SH, et al. Bone probing measurement as a reliable evaluation of the bone level in periodontal defects. J Periodontol 2000;71:729.
Bone Replacement Grafts 7176. Eickholz P, Kim TS, Benn DK, et al. Validity of radiographic measurement of interproximal bone loss. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 1998;85:99.77. Carranza FA Jr, Jolkovsky DL. Current status of periodontal therapy for furcation involvements. Dent Clin North Am 1991;35:555.78. Laurell L, Gottlow J, Zybutz M, et al. Treatment of intrabony defects by different surgical procedures. A literature review. J Periodontol 1998;69:303.79. Cortellini P, Bowers GM. Periodontal regeneration of intrabony defects: an evidence-based treatment approach. Int J Periodontics Restorative Dent 1995; 15:128.80. Bowers GM, Schallhorn RG, McClain PK, et al. Factors influencing the outcome of regenerative therapy in mandibular Class II furcations: part I. J Periodontol 2003; 74:1255.81. Needleman I, Tucker R, Giedrys-Leeper E, et al. A systematic review of guided tissue regeneration for periodontal infrabony defects. J Periodontal Res 2002; 37:380.82. Trombelli L, Heitz-Mayfield LJ, Needleman I, et al. A systematic review of graft materials and biological agents for periodontal intraosseous defects. J Clin Perio- dontol 2002;29(Suppl 3):117.83. Trombelli L. Which reconstructive procedures are effective for treating the periodontal intraosseous defect? Periodontol 2000 2005;37:88.84. Brunsvold MA, Mellonig JT. Bone grafts and periodontal regeneration. Periodon- tol 2000 1993;1:80.85. Yukna R, Salinas TJ, Carr RF. Periodontal regeneration following use of ABM/P-1 5: a case report. Int J Periodontics Restorative Dent 2002;22:146.86. Hartman GA, Arnold RM, Mills MP, et al. Clinical and histologic evaluation of anor- ganic bovine bone collagen with or without a collagen barrier. Int J Periodontics Restorative Dent 2004;24:127.87. Ridgway HK, Mellonig JT, Cochran DL. Human histologic and clinical evaluation of recombinant human platelet-derived growth factor and beta-tricalcium phos- phate for the treatment of periodontal intraosseous defects. Int J Periodontics Restorative Dent 2008;28:171.88. Garrett S. Periodontal regeneration around natural teeth. Ann Periodontol 1996;1: 621.89. Wang HL, Cooke J. Periodontal regeneration techniques for treatment of periodontal diseases. Dent Clin North Am 2005;49:637.90. Aichelmann-Reidy ME, Reynolds MA. Predictability of clinical outcomes following regenerative therapy in intrabony defects. J Periodontol 2008;79:387.91. Rosen PS, Marks MH, Reynolds MA. Influence of smoking on long-term clinical results of intrabony defects treated with regenerative therapy. J Periodontol 1996;67:1159.92. Johnson GK, Hill M. Cigarette smoking and the periodontal patient. J Periodontol 2004;75:196.93. Nevins M, Giannobile WV, McGuire MK, et al. Platelet-derived growth factor stim- ulates bone fill and rate of attachment level gain: results of a large multicenter randomized controlled trial. J Periodontol 2005;76:2205.